Laboratory 4 Bending Test of Materials

 Teresa Simon
 6 months ago
 Views:
Transcription
1 Department of Materials and Metallurgical Engineering Bangladesh University of Engineering Technology, Dhaka MME 222 Materials Testing Sessional.50 Credits Laboratory 4 Bending Test of Materials. Objective Bend or flexure testing is common in springs and brittle materials whose failure behaviours are linear such as concretes, stones, woods, plastics, glasses and ceramics. Other types of brittle materials such as powder metallurgy processed metals and materials are normally tested under a transverse flexure. Bend test is therefore suitable for evaluating strength of brittle materials where conduction of tensile test and interpretation of test result of material is difficult and sometimes impossible. After completion of this experiment, students should be able to. conduct 3point bend test and investigate responses of materials when subjected to bending.2 determine flexural bend strength and elastic modulus of brittle material, and.3 analyse statistical nature of the test data and determine the Weibull modulus of the brittle materials 2. Materials and Equipment 2. Bend samples 2.2 Universal testing machine 2.3 Vernia calliper 3. Experimental Procedure 3. Bend test of materials 3.. Measure the width and thickness of the specimen. Mark on the locations where the load will be applied under threepoint bending Place the sample carefully on to the stage of 3point bending fixture of a universal testing machine. Make sure that the loading point is placed on to the marked location Carry out the bend test until failure takes place Construct the loadextension or loaddeflection curve to calculate the flexural bend strength and elastic modulus of the specimen Repeat steps 3.. to 3..4 to conduct bend tests of other specimens. 3.7 Complete the Data Sheet, Table Statistical analysis of data 3.2. Conduct 3point bend test of at least 5 glass specimens following steps 3.. to Note the breaking loads and then determine flexural bend strength (MOR) of these specimens.
2 3.2.3 Arrange them in descending order, rank them and determine their failure probability, P f Construct ln ( ln ( P f )) vs. ln (MOR) curve and determine Weibull constants m and Results 4. Display the test data in the Table. 4.2 Determine bend strength, elastic modulus and flexural strength (MOR) of the material. 4.3 Determine Weibul modulus of the material and comment on the degree of homogeneity of the material. 5. Discussion 5. Answer the following questions: (a) Give three examples of engineering applications that involve bending properties of materials. (b) What would you expect if the bending experiment has been carried out at elevated temperature? (c) Why does the presence of cracks in ductile materials present not much problem when compare with brittle material? (d) Explain why flexural strength of brittle material is always higher than tensile strength of the respective material. (e) (f) Determine the flexural strength of material testing using 4point bend test. What conclusion can you draw from the Weibull modulus value of a test sample? (g) Compare and explain the Weibull modulus of cast and wrought aluminium alloys. 2
3 Table 3.: Data Sheet for Bend Test Sample identification Symbol Unit Value 2 3 Average Material Width of sample w mm Thickness of sample t mm Span length of sample L mm Fracture load P f kn Flexural Bend Strength (MOR) fb MPa Elastic Modulus E b GPa **Provide all calculations in separate pages. Signature with Date of the Instructor/Course Tutor 3
4 6.0 Theoretical Background 6. Introduction Preparing specimens from brittle materials, such as ceramics and glasses, for direct tension tests is difficult because of the problems involved in shaping and machining them to proper dimensions. Furthermore, such specimens are sensitive to surface defects and notches, and clamping brittle test specimens for testing is difficult. Also, improper alignment of the test specimen may result in a nonuniform stress distribution along the cross section and ultimate premature failure. A commonly used test method for measuring strength of brittle materials such as ceramics and glasses is the bend or flexure test. The test specimen can have a circular, square, or rectangular cross section and is uniform along the complete length. Such a specimen is much less expensive to fabricate than a tensile specimen. The test is conducted with the same kind of universal testing machine used for tensile and compressive strength measurements. The test specimen is supported at the ends and the load is applied either at the centre (threepoint loading) or at two positions (fourpoint loading), Fig. 6.. The longitudinal stresses in the specimens are tensile at their lower surfaces and compressive at their upper surfaces. The bend or flexural strength is defined as the maximum uniaxial tensile strength at failure and it is often referred to as the flexural strength or modulus of rupture (MOR). P P/2 P/2 L/2 P/2 L P/2 c = t/2 a P/2 L P/2 c = t/2 (a) Figure 6.: Two bendtest methods for brittle materials: (a) threepoint bending; (b) fourpoint bending. The areas on the beams represent the bending moment diagrams. Note the region of constant maximum bending moment in (b); by contrast, the maximum bending moment occurs only at the centre of the specimen in (a). (b) Threepoint testing is still an option, but fourpoint is preferred since more material is exposed to high stress. Also, because of the larger volume of material subjected to the same bending moment in Fig. 6.b, there is a higher probability that defects exist in this volume than in that in Fig. 6.a. Consequently, the fourpoint test gives a lower modulus of rupture than the threepoint test. Figure 6.2 illustrates threepoint bending arrangement which is capable of 80 bend angle for welded materials. 6.2 ThreePoint Bend Test of Brittle Materials Considering a three point bend test of an elastic material, when the load P is applied at the midspan of specimen in an xy plane, stress distribution across the specimen thickness (t) is demonstrated in Fig The stress is essentially zero at the neutral axis NN. Stresses in the y axis in the positive direction represent tensile stresses whereas stresses in the negative direction represent compressive stresses. Within the elastic range, brittle materials show a linear relationship of load and deflection where yielding occurs on a thin layer of the 4
5 Figure 6.2: Example of a weld plate bend tested under a threepoint bend arrangement. specimen surface at the midspan, Fig. 6.3a. This in turn leads to crack initiation which finally proceeds to specimen failure. Ductile materials however provide loaddeflection curves which deviate from a linear relationship before failure takes place as opposed to those of brittle materials previously mentioned. Furthermore, it is also difficult to determine the beginning of yielding in this case. The stress distribution of a ductile material after yielding is given in Fig. 6.3b. Therefore, it can be seen that bend testing is not suitable for ductile materials due to difficulties in determining the yield point of the materials under bending and the obtained stressstrain curve in the elastic region may not be linear. The results obtained might not be validated. As a result, the bend test is therefore more appropriate for testing brittle materials whose stressstrain curves (Fig. 6.4) show its linear elastic behaviour just before the materials fail. P w x P/2 z y P/2 c c t/2 t/2 t/2 t/2 c c (a) Figure 6.3: Stress distributions in a rectangular bar when (a) elastically bended and (b) after yielding (b) 5
6 Figure 6.4: Flexural stress and flexural strain relationship Determination of flexural strength and elastic modulus For a beam in flexure, the maximum outer fibre stress from simple beam theory is: σ fb = M c I where M is the applied moment, c is the distance of the outer fibres (where the tensile force is acting) from the neutral axis, and I is the moment of inertia of the cross section about the neutral axis. It is assumed that the material behaviour is consistent with Hooke s law. For a rectangular test specimen I = bt 3 /2 and c = t/2, where b and t are the width and thickness of the specimen, respectively. With reference to 3point a configurations, Fig. 6.4, the bending moment can be calculated as M = Replacing the values of M, c and I in eq.(6.) to obtain the flexural bending strength σ fb = P L 4 (6.) (6.2) 3PL 2bt 2 (6.3) From the experimental result, we can also obtain the elastic modulus of the material according to the linearelastic analysis. The deflection of the beam () from the centre as illustrated in Fig. 6.3 can be expressed as δ = PL 3 48 E I where I = wt 3 2. The elastic modulus (E B ) in the above equation can be calculated from the slope of the loaddeflection curve (dp/d) in the linear region as follows (6.4) E B = L 3 48 I (dp dδ ) (6.5) E B = m L 3 (6.6) 4 w t 3 where m = (dp/d) is the slope of the tangent to the straightline portion of the loaddeflection beam. 6
7 6.3 The Weibull modulus The strength characterisation data of ceramics reported in terms of flexural bend strength or MOR is relatively inexpensive, straightforward and quick process. But it has severe limitation on the usability of MOR data: the measured strength varies significantly depending on the size of the specimen tested and whether it is loaded in threepoint or fourpoint. Ceramics do not have uniquely defined failure strength. A given batch of ceramic specimens usually does not show a constant measured strength instead they show a range of strengths. The strength of ceramic is determined by a combination of two material parameters the toughness and the crack size. Since fracture toughness is not a variable, the variation in strength comes from a variation in the size of the largest defect (crack), Fig. 6.5, and the microstructure. There are lots of small defects, besides the largest ones, present in the material which are stressed but they do not reach their critical stress for propagation. Hence, it is necessary to use sample sets of ten or more specimens for even the simplest of goals such as determining an average strength for material ranking, material development, or materials specification purposes and a probabilistic approach is needed to interpret test data. Thus, it is also widely recognized that brittle material strengths are statistical in nature. Largest defect Figure 6.4: Flaw distribution in ceramic materials. When analysing the variation in the strength of ceramics, a particular function, due to the Swedish engineer Weibull, has been found to be useful. The simplest form of Weibull approach of characterising the flaw distribution is based on a weakest link model and it is analogous to the breaking of a length of chain. Failure occurs when the weakest link breaks. In a series of chains of a particular length, the weakest link in each length is of different strength and this controls the variation in strength. In ceramics, the links could represent small volumes of material containing a flaw and the weakest link is equivalent to the region with the largest flaw. Considering the twoparameter model, the probability of some length L of a link failing at a stress is P f = P s = exp { ( σ m ) } (6.7) σ 0 Where P f and P s are, respectively, the probability of failure and survival, 0 is a constant called the normalising stress, and m is a number, usually referred to as the Weibull modulus, which reflects the degree of variability in strength the higher the m is, the less variable is the strength. In this Weibull function, the Weibull modulus, m, defines the shape of the failure distribution curve. If m tends to be zero, the failure probability tends to become independent of the applied stress. If m =, the failure probability becomes a simple asymptotic exponential distribution. If m =, the distribution is a step function with P f = 0 when < 0, and P f = when > 0. P f P f m = m = 0 0 7
8 The Weibull modulus, m, also defines the width of the probability distribution, Fig If m is large, the distribution is narrow showing a small spread of failure strength, indicating high reliability of the material. If, on the other hand, m is small, the distribution is wide showing a large variation in the failure strength, indicating unreliability of the material. Poor ceramics have m in the range of 3 0, while good engineering ceramics have m in the range 0 40, and homogeneous metals and alloys have m well above 00. P f P f large m small m 0 0 A substantial number of test samples are required to determine accurate value for the Weibull slope m. Testing of only 0 samples can result in an error as high as ±40% in the m value. Over 80 samples are required to obtain 90% confidence in the m value Determining Weibull parameters from experimental data Taking natural logarithms in both sides of eq.(3.7), we get ln P s = ( σ m ) σ 0 (6.8) Taking natural logarithms again ln ( ln P s ) = m ln σ m ln σ 0 (6.9) ln { ln( P f )} = m ln σ m ln σ 0 (6.0) Thus plotting ln ( ln P s ) or ln ( ln ( P f ) as ordinate against ln as abscissa should give a straight line of the form y = mc + c. Here the gradient of the equation is the Weibull modulus m and the intercept to yaxis is the normalising stress 0 in the form of m ln 0. In the analysis of a number of strength data of a typical material through Weibull statistics, the plotting positions for abscissa are obvious but not the ordinate. The failure probability at a given stress is found by first ranking the failure stresses in order of strength. The failure probability of nth ranked sample from a total of N would be P f =( P s ) =n/(n+). The figure shown below is a Weibull plot of nine fracture strength data of abraded glass rods. The Weibull modulus of the sample is 4.76, indicating very poor reliability of the data. 8
Chapter 7. Highlights:
Chapter 7 Highlights: 1. Understand the basic concepts of engineering stress and strain, yield strength, tensile strength, Young's(elastic) modulus, ductility, toughness, resilience, true stress and true
More informationUNIT I SIMPLE STRESSES AND STRAINS
Subject with Code : SM1(15A01303) Year & Sem: IIB.Tech & ISem SIDDHARTH GROUP OF INSTITUTIONS :: PUTTUR Siddharth Nagar, Narayanavanam Road 517583 QUESTION BANK (DESCRIPTIVE) UNIT I SIMPLE STRESSES
More informationIntroduction to Engineering Materials ENGR2000. Dr. Coates
Introduction to Engineering Materials ENGR2 Chapter 6: Mechanical Properties of Metals Dr. Coates 6.2 Concepts of Stress and Strain tension compression shear torsion Tension Tests The specimen is deformed
More informationMeasurement of Bone Strength and Stiffness using 3Point Bending
BME 315 Biomechanics, U. Wisconsin Adapted by R. Lakes from D. Thelen and C. Decker, 09, adapted from Lakes 06 Experimental Details I. Laboratory equipment The load frame that we will use to perform our
More informationTuesday, February 11, Chapter 3. Load and Stress Analysis. Dr. Mohammad Suliman Abuhaiba, PE
1 Chapter 3 Load and Stress Analysis 2 Chapter Outline Equilibrium & FreeBody Diagrams Shear Force and Bending Moments in Beams Singularity Functions Stress Cartesian Stress Components Mohr s Circle for
More informationPhysical Properties Testing Technical Bulletin
Technical Bulletin MANUFACTURER Raven Lining Systems 13105 E. 61 st Street, Suite A Broken Arrow, OK 74012 (918) 6150020 TENSILE TESTING OF PLASTICS ASTM D638, ISO 527 Tensile tests measure the force
More informationFlexure: Behavior and Nominal Strength of Beam Sections
4 5000 4000 (increased d ) (increased f (increased A s or f y ) c or b) Flexure: Behavior and Nominal Strength of Beam Sections Moment (kipin.) 3000 2000 1000 0 0 (basic) (A s 0.5A s ) 0.0005 0.001 0.0015
More informationTINIUS OLSEN Testing Machine Co., Inc.
Interpretation of StressStrain Curves and Mechanical Properties of Materials Tinius Olsen has prepared this general introduction to the interpretation of stressstrain curves for the benefit of those
More informationMECHANICAL PROPERTIES OF SOLIDS
Chapter Nine MECHANICAL PROPERTIES OF SOLIDS MCQ I 9.1 Modulus of rigidity of ideal liquids is (a) infinity. (b) zero. (c) unity. (d) some finite small nonzero constant value. 9. The maximum load a wire
More informationCivil Engineering Design (1) Design of Reinforced Concrete Columns 2006/7
Civil Engineering Design (1) Design of Reinforced Concrete Columns 2006/7 Dr. Colin Caprani, Chartered Engineer 1 Contents 1. Introduction... 3 1.1 Background... 3 1.2 Failure Modes... 5 1.3 Design Aspects...
More information2. Rigid bar ABC supports a weight of W = 50 kn. Bar ABC is pinned at A and supported at B by rod (1). What is the axial force in rod (1)?
IDE 110 S08 Test 1 Name: 1. Determine the internal axial forces in segments (1), (2) and (3). (a) N 1 = kn (b) N 2 = kn (c) N 3 = kn 2. Rigid bar ABC supports a weight of W = 50 kn. Bar ABC is pinned at
More informationLab Exercise #3: Torsion
Lab Exercise #3: Prelab assignment: Yes No Goals: 1. To evaluate the equations of angular displacement, shear stress, and shear strain for a shaft undergoing torsional stress. Principles: testing of round
More informationCHAPTER 6 BENDING Part 1
Ishik University / Sulaimani Civil Engineering Department Mechanics of Materials CE 211 CHAPTER 6 BENDING Part 11 CHAPTER 6 Bending Outlines of this chapter: 6.1. Chapter Objectives 6.2. Shear and
More information= 50 ksi. The maximum beam deflection Δ max is not = R B. = 30 kips. Notes for Strength of Materials, ET 200
Notes for Strength of Materials, ET 00 Steel Six Easy Steps Steel beam design is about selecting the lightest steel beam that will support the load without exceeding the bending strength or shear strength
More informationFracture Behavior. Section
Section 6 Fracture Behavior In January 1943 the oneday old Liberty Ship, SS Schenectady, had just completed successful sea trials and returned to harbor in calm cool weather when... "Without warning and
More informationPLATE GIRDERS II. Load. Web plate Welds A Longitudinal elevation. Fig. 1 A typical Plate Girder
16 PLATE GIRDERS II 1.0 INTRODUCTION This chapter describes the current practice for the design of plate girders adopting meaningful simplifications of the equations derived in the chapter on Plate Girders
More informationJournal of Composite Materials. Behaviour of hollow pultruded GFRP square beams with different shear spantodepth ratios
Behaviour of hollow pultruded GFRP square beams with different shear spantodepth ratios Journal: Manuscript ID: Draft Manuscript Type: Original Manuscript Date Submitted by the Author: n/a Complete List
More informationASSESSMENT OF DYNAMICALLY LOADED CRACKS IN FILLETS
ASSESSMENT OF DNAMICALL LOADED CRACKS IN FILLETS Uwe Zencker, Linan Qiao, Bernhard Droste Federal Institute for Materials Research and Testing (BAM) 12200 Berlin, Germany email: zencker@web.de Abstract
More informationstructural analysis Excessive beam deflection can be seen as a mode of failure.
Structure Analysis I Chapter 8 Deflections Introduction Calculation of deflections is an important part of structural analysis Excessive beam deflection can be seen as a mode of failure. Extensive glass
More informationUnified Quiz M4 May 7, 2008 M  PORTION
9:0010: 00 (last four digits) 32141 Unified Quiz M4 May 7, 2008 M  PORTION Put the last four digits of your MIT ID # on each page of the exam. Read all questions carefully. Do all work on that question
More informationA PROTOCOL FOR DETERMINATION OF THE ADHESIVE FRACTURE TOUGHNESS OF FLEXIBLE LAMINATES BY PEEL TESTING: FIXED ARM AND TPEEL METHODS
1 A PROTOCOL FOR DETERMINATION OF THE ADHESIVE FRACTURE TOUGHNESS OF FLEXIBLE LAMINATES BY PEEL TESTING: FIXED ARM AND TPEEL METHODS An ESIS Protocol Revised June 2007, Nov 2010 D R Moore, J G Williams
More informationASPECTS CONCERNING TO THE MECHANICAL PROPERTIES OF THE GLASS / FLAX / EPOXY COMPOSITE MATERIAL
5 th International Conference Advanced Composite Materials Engineering COMAT 2014 1617 October 2014, Braşov, Romania ASPECTS CONCERNING TO THE MECHANICAL PROPERTIES OF THE GLASS / FLAX / EPOXY COMPOSITE
More informationChapter 6: Mechanical Properties of Metals. Dr. Feras Fraige
Chapter 6: Mechanical Properties of Metals Dr. Feras Fraige Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility Toughness
More informationMECH 344/X Machine Element Design
1 MECH 344/X Machine Element Design Time: M 14:4517:30 Lecture 2 Contents of today's lecture Introduction to Static Stresses Axial, Shear and Torsional Loading Bending in Straight and Curved Beams Transverse
More informationD e s i g n o f R i v e t e d J o i n t s, C o t t e r & K n u c k l e J o i n t s
D e s i g n o f R i v e t e d J o i n t s, C o t t e r & K n u c k l e J o i n t s 1. Design of various types of riveted joints under different static loading conditions, eccentrically loaded riveted joints.
More informationBridge deck modelling and design process for bridges
EURussia Regulatory Dialogue Construction Sector Subgroup 1 Bridge deck modelling and design process for bridges Application to a composite twingirder bridge according to Eurocode 4 Laurence Davaine
More informationBasis of Structural Design
Basis of Structural Design Course 2 Structural action: cables and arches Course notes are available for download at http://www.ct.upt.ro/users/aurelstratan/ Structural action Structural action: the way
More informationChapter kn m/kg Ans kn m/kg Ans. 187 kn m/kg Ans.
Chapter 1 From Tables A0, A1, A, and A4c, (a) UNS G1000 HR: S ut = 80 (55) MPa (kpsi), S yt = 10 (0) MPa (kpsi) Ans. (b) SAE 1050 CD: S ut = 690 (100) MPa (kpsi), S yt = 580 (84) MPa (kpsi) Ans. (c)
More informationA STUDY ON FATIGUE CRACK GROWTH IN CONCRETE IN THE PREPARIS REGION
VIII International Conference on Fracture Mechanics of Concrete and Concrete Structures FraMCoS8 J.G.M. Van Mier, G. Ruiz, C. Andrade, R.C. Yu and X.X. Zhang (Eds) A STUDY ON FATIGUE CRACK GROWTH IN CONCRETE
More informationTMHL TMHL (Del I, teori; 1 p.) SOLUTION I. II.. III. Fig. 1.1
TMHL6 2040830 (Del I, teori; p.). Fig.. shows three cases of sharp cracks in a sheet of metal. In all three cases, the sheet is assumed to be very large in comparison with the crack. Note the different
More informationMechanics of Materials MENG 270 Fall 2003 Exam 3 Time allowed: 90min. Q.1(a) Q.1 (b) Q.2 Q.3 Q.4 Total
Mechanics of Materials MENG 70 Fall 00 Eam Time allowed: 90min Name. Computer No. Q.(a) Q. (b) Q. Q. Q.4 Total Problem No. (a) [5Points] An air vessel is 500 mm average diameter and 0 mm thickness, the
More informationCONSTITUTIVE RELATIONS FOR LINEAR ELASTIC SOLIDS
Chapter 9 CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS Figure 9.1: Hooke memorial window, St. Helen s, Bishopsgate, City of London 211 212 CHAPTR 9. CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS 9.1 Mechanical
More informationDesign of Glass Panes for Uniformly Distributed Loads
Design of Glass Panes for Uniformly Distributed Loads Miguel Rui Sousa de Almeida Mechanical Engineering Department, Instituto Superior Técnico, Av. Rovisco Pais, 1049001 Lisboa, Portugal Email : miguelrui412@gmail.com
More informationFatigue Resistance of Angle Shape Shear Connector used in SteelConcrete Composite Slab
Fatigue Resistance of Angle Shape Shear Connector used in SteelConcrete Composite Slab A dissertation submitted to the Graduate School of Engineering of Nagoya University in partial fulfillment of the
More informationAutodesk Robot Structural Analysis Professional 2014 Design of fixed beamtocolumn connection EN :2005/AC:2009
Autodesk Robot Structural Analysis Professional 2014 Design of fixed beamtocolumn connection EN 199318:2005/AC:2009 Ratio 0,44 GENERAL Connection no.: 24 Connection name: Ligação 2 Structure node:
More informationSERVICEABILITY LIMIT STATE DESIGN
CHAPTER 11 SERVICEABILITY LIMIT STATE DESIGN Article 49. Cracking Limit State 49.1 General considerations In the case of verifications relating to Cracking Limit State, the effects of actions comprise
More information4. SHAFTS. A shaft is an element used to transmit power and torque, and it can support
4. SHAFTS A shaft is an element used to transmit power and torque, and it can support reverse bending (fatigue). Most shafts have circular cross sections, either solid or tubular. The difference between
More informationS HEAR S TRENGTH IN P RINCIPAL P LANE OF W OOD
S HEAR S TRENGTH IN P RINCIPAL P LANE OF W OOD By Jen Y. Liu 1 and Lester H. Floeter 2 ABSTRACT: In this study, the writers used Tsai and Wu s tensor polynomial theory to rederive a formula originally
More informationPullout Tests of Geogrids Embedded in Noncohesive Soil
Archives of HydroEngineering and Environmental Mechanics Vol. 51 (2004), No. 2, pp. 135 147 Pullout Tests of Geogrids Embedded in Noncohesive Soil Angelika Duszyńska, Adam F. Bolt Gdansk University of
More information6.37 Determine the modulus of resilience for each of the following alloys:
6.37 Determine the modulus of resilience for each of the following alloys: Yield Strength Material MPa psi Steel alloy 550 80,000 Brass alloy 350 50,750 Aluminum alloy 50 36,50 Titanium alloy 800 116,000
More informationAnisotropic modeling of short fibers reinforced thermoplastics materials with LSDYNA
Anisotropic modeling of short fibers reinforced thermoplastics materials with LSDYNA Alexandre Hatt 1 1 Faurecia Automotive Seating, Simplified Limited Liability Company 1 Abstract / Summary Polymer thermoplastics
More informationDETERMINING THE STRESS PATTERN IN THE HH RAILROAD TIES DUE TO DYNAMIC LOADS 1
PERIODICA POLYTECHNICA SER. CIV. ENG. VOL. 46, NO. 1, PP. 125 148 (2002) DETERMINING THE STRESS PATTERN IN THE HH RAILROAD TIES DUE TO DYNAMIC LOADS 1 Nándor LIEGNER Department of Highway and Railway Engineering
More information1.050 Content overview Engineering Mechanics I Content overview. Selection of boundary conditions: Euler buckling.
.050 Content overview.050 Engineering Mechanics I Lecture 34 How things fail and how to avoid it Additional notes energy approach I. Dimensional analysis. On monsters, mice and mushrooms Lectures 3. Similarity
More informationUNIVERSITÀ DEGLI STUDI DI PADOVA DIPARTIMENTO DI INGEGNERIA CIVILE, EDILE ED AMBIENTALE CORSO DI LAUREA MAGISTRALE IN INGEGNERIA CIVILE
UNIVERSITÀ DEGLI STUDI DI PADOVA DIPARTIMENTO DI INGEGNERIA CIVILE, EDILE ED AMBIENTALE CORSO DI LAUREA MAGISTRALE IN INGEGNERIA CIVILE Tesi di laurea Magistrale in Ingegneria Civile Curriculum Strutture
More informationFRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING.
FRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING. X. J. Gong, F. Hernandez, G. Verchery. ISAT  Institut Supérieur de l Automobile et des Transports, LRMA  Laboratoire de
More informationDETERMINATION OF EI FOR PULTRUDED GFRP SHEET PILE PANELS. Abstract
DETERMINATION OF EI FOR PULTRUDED GFRP SHEET PILE PANELS Yixin Shao, Cynthia Giroux and Zeid Bdeir McGill University Montreal, Quebec, Canada Abstract The flexural rigidity, EI, plays an especially important
More informationSANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS
SANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS de Aguiar, José M., josemaguiar@gmail.com Faculdade de Tecnologia de São Paulo, FATECSP Centro Estadual de Educação Tecnológica Paula Souza. CEETEPS
More informationIntroduction to Continuous Systems. Continuous Systems. Strings, Torsional Rods and Beams.
Outline of Continuous Systems. Introduction to Continuous Systems. Continuous Systems. Strings, Torsional Rods and Beams. Vibrations of Flexible Strings. Torsional Vibration of Rods. BernoulliEuler Beams.
More informationVALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 )
VALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 ) Graham D Sims and William R Broughton Composites Design Data and Methods, Centre for Materials
More informationSTRUCTURAL ANALYSIS CHAPTER 2. Introduction
CHAPTER 2 STRUCTURAL ANALYSIS Introduction The primary purpose of structural analysis is to establish the distribution of internal forces and moments over the whole part of a structure and to identify
More informationAmerican Earthquake Joint System for Resistance to EarthquakeInduced Ground Deformation
American Earthquake Joint System for Resistance to EarthquakeInduced Ground Deformation Final Report Submitted to: Mr. David Drake American Cast Iron Pipe Company P.O. Box 2727 Birmingham, AL 35202 USA
More informationElastic and ElasticPlastic Behaviour of a Crack in a Residual Stress Field
Residual Stresses 2016: IC10 Elastic and ElasticPlastic Behaviour of a Crack in a Residual Stress Field Guiyi Wu a, Chris Aird b, David Smith and Martyn Pavier c* Department of Mechanical Engineering,
More informationPressure Vessels Stresses Under Combined Loads Yield Criteria for Ductile Materials and Fracture Criteria for Brittle Materials
Pressure Vessels Stresses Under Combined Loads Yield Criteria for Ductile Materials and Fracture Criteria for Brittle Materials Pressure Vessels: In the previous lectures we have discussed elements subjected
More informationBeam Bending Stresses and Shear Stress
Beam Bending Stresses and Shear Stress Notation: A = name or area Aweb = area o the web o a wide lange section b = width o a rectangle = total width o material at a horizontal section c = largest distance
More informationParametric analysis and torsion design charts for axially restrained RC beams
Structural Engineering and Mechanics, Vol. 55, No. 1 (2015) 127 DOI: http://dx.doi.org/10.12989/sem.2015.55.1.001 1 Parametric analysis and torsion design charts for axially restrained RC beams Luís F.A.
More informationReliable Test Results
Intelligent testing Johannes J.Bührle  Agenda Reliable test results are a fundamental and highly topical aspect of materials testing. Using suitable examples we would like to show you how we view this
More information999 TOWN & COUNTRY ROAD ORANGE, CALIFORNIA TITLE PUSHOVER ANALYSIS EXAMPLE BY R. MATTHEWS DATE 5/21/01
DESCRIPTION Nonlinear static (pushover) analysis will be performed on a railroad bridge bent using several methods to determine its ultimate lateral deflection capability. 1. SAP2000 Nonlinear with axialmoment
More informationSpherical Pressure Vessels
Spherical Pressure Vessels Pressure vessels are closed structures containing liquids or gases under essure. Examples include tanks, pipes, essurized cabins, etc. Shell structures : When essure vessels
More informationDesign of reinforced concrete sections according to EN and EN
Design of reinforced concrete sections according to EN 199211 and EN 19922 Validation Examples Brno, 21.10.2010 IDEA RS s.r.o. South Moravian Innovation Centre, U Vodarny 2a, 616 00 BRNO tel.: +420511
More informationChapter 8 BIAXIAL BENDING
Chapter 8 BAXAL BENDN 8.1 DEFNTON A cross section is subjected to biaial (oblique) bending if the normal (direct) stresses from section are reduced to two bending moments and. enerall oblique bending is
More informationThe Effects of Holesize and Environment on the Mechanical Behaviour of a Quasiisotropic AS4/ Laminate in Tension, Compression and Bending
The Effects of Holesize and Environment on the Mechanical Behaviour of a Quasiisotropic AS4/3506 Laminate in Tension, Compression and Bending Paul J. Callus Air Vehicles Division Defence Science and
More informationElasticPlastic Fracture Mechanics. Professor S. Suresh
ElasticPlastic Fracture Mechanics Professor S. Suresh Elastic Plastic Fracture Previously, we have analyzed problems in which the plastic zone was small compared to the specimen dimensions (small scale
More informationBehavior and Modeling of Existing Reinforced Concrete Columns
Behavior and Modeling of Existing Reinforced Concrete Columns Kenneth J. Elwood University of British Columbia with contributions from Jose Pincheira, Univ of Wisconsin John Wallace, UCLA Questions? What
More informationBME 207 Introduction to Biomechanics Spring 2017
April 7, 2017 UNIVERSITY OF RHODE ISAND Department of Electrical, Computer and Biomedical Engineering BE 207 Introduction to Biomechanics Spring 2017 Homework 7 Problem 14.3 in the textbook. In addition
More informationMECHANICS OF SOLIDS Credit Hours: 6
MECHANICS OF SOLIDS Credit Hours: 6 Teaching Scheme Theory Tutorials Practical Total Credit Hours/week 4 0 6 6 Marks 00 0 50 50 6 A. Objective of the Course: Objectives of introducing this subject at second
More informationQuestion 1. Ignore bottom surface. Solution: Design variables: X = (R, H) Objective function: maximize volume, πr 2 H OR Minimize, f(x) = πr 2 H
Question 1 (Problem 2.3 of rora s Introduction to Optimum Design): Design a beer mug, shown in fig, to hold as much beer as possible. The height and radius of the mug should be not more than 20 cm. The
More informationCOMPUTER AIDED DESIGN IN CASE OF THE LAMINATED COMPOSITE MATERIALS
6 th International Conference Computational Mechanics and Virtual Engineering COMEC 15 1516 October 15, Braşov, Romania COMPUER AIDED DESIGN IN CASE OF HE LAMINAED COMPOSIE MAERIALS Camelia Cerbu ransilvania
More informationApplication of a nonlocal failure criterion to a crack in heterogeneous media S. Bavaglia*, S.E. Mikhailov*
Application of a nonlocal failure criterion to a crack in heterogeneous media S. Bavaglia*, S.E. Mikhailov* University of Perugia, Italy Email: mic@unipg.it ^Wessex Institute of Technology, Ashurst Lodge,
More informationEFFECT OF CONCRETE CRUSHING ON FLEXURAL STRENGTH OF STEELCONCRETE COMPOSITE GIRDERS
EFFECT OF CONCRETE CRUSHING ON FLEXURAL STRENGTH OF STEELCONCRETE COMPOSITE GIRDERS Vivek Kumar GUPTA 1, Yoshiaki OKUI 2, Naofumi INABA 3 and Masatsugu NAGAI 4 1 Member of JSCE, Lead Structural Engineer,
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationCharpy VNotch Impact Testing
Charpy VNotch Impact Testing ENGR45 Materials Science Laboratory Chad Philip Johnson Submitted: May 15 th 2013 Abstract The Charpy Vnotch test is an engineering method that is frequently used to measure
More informationModulus Of Elasticity And Poissons Ratio
And Poissons Ratio Free PDF ebook Download: And Poissons Ratio Download or Read Online ebook modulus of elasticity and poissons ratio in PDF Format From The Best User Guide Database ASTM C 469, the Standard
More informationThe Influence of Discontinuities on Elastic and Mechanical Properties of Composite Materials Reinforced with Woven Carbon, Carbonkevlar and Kevlar
The Influence of Discontinuities on Elastic and Mechanical Properties of Composite Materials Reinforced with Woven Carbon, Carbonkevlar and Kevlar DUMITRU BOLCU 1 *, MIHAELA SAVA 2, ALIN DINITA 3, COSMIN
More informationOPTIMISING THE MECHANICAL CHARACTERISATION OF A RESILIENT INTERLAYER FOR THE USE IN TIMBER CON STRUCTION
OPTIMISING THE MECHANICAL CHARACTERISATION OF A RESILIENT INTERLAYER FOR THE USE IN TIMBER CON STRUCTION Luca Barbaresi, Federica Morandi, Juri Belcari, Andrea Zucchelli and Alice Speranza University
More informationGiorgio Mattei. 31 March 2016
Giorgio Mattei giorgio.mattei@centropiaggio.unipi.it 31 March 2016 StressStrain curve is the relationship between the stress and the strain exhibited by a given material. It is unique for each material
More informationModule 5. Flanged Beams Theory and Numerical Problems. Version 2 CE IIT, Kharagpur
Module 5 Flanged Beams Theory and Numerical Problems Lesson 10 Flanged Beams Theory Instructional Objectives: At the end of this lesson, the student should be able to: identify the regions where the beam
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationAvailable online at ScienceDirect. Procedia Engineering 172 (2017 )
Available online at www.sciencedirect.com ScienceDirect Procedia Engineering 172 (2017 ) 1093 1101 Modern Building Materials, Structures and Techniques, MBMST 2016 Iterative Methods of BeamStructure Analysis
More informationStudy of the Evolution of Elastoplastic Zone by Volumetric Method
International Journal of Mechanics and Applications 2015, 5(1): 19 DOI: 10.5923/j.mechanics.20150501.01 Study of the Evolution of Elastoplastic Zone by Volumetric Method M. Moussaoui 1,*, S. Meziani 2
More informationElastic moduli: Overview and characterization methods
Technical Review ITCME/ATCP Elastic moduli: Overview and characterization methods ATCP Physical Engineering www.atcpndt.com Authors: Leiliane Cristina Cossolino (Cossolino LC) and Antônio Henrique Alves
More informationEffects of geometric and material parameters on failure modes of SC elements
Aalto University School of Engineering Department of Mechanical Engineering Vishesh Lohani Effects of geometric and material parameters on failure modes of SC elements Thesis submitted in partial fulfilment
More informationIntensity (a.u.) Intensity (a.u.) Raman Shift (cm 1 ) Oxygen plasma. 6 cm. 9 cm. 1mm. Singlelayer graphene sheet. 10mm. 14 cm
Intensity (a.u.) Intensity (a.u.) a Oxygen plasma b 6 cm 1mm 10mm Singlelayer graphene sheet 14 cm 9 cm Flipped Si/SiO 2 Patterned chip Plasmacleaned glass slides c d After 1 sec normal Oxygen plasma
More informationTheory and Analysis of Structures
7 Theory and nalysis of Structures J.Y. Richard iew National University of Singapore N.E. Shanmugam National University of Singapore 7. Fundamental Principles oundary Conditions oads and Reactions Principle
More informationModeling of the Bending Stiffness of a Bimaterial Beam by the Approximation of OneDimensional of Laminated Theory
. FloresDomínguez Int. Journal of Engineering Research and Applications RESEARCH ARTICLE OPEN ACCESS odeling of the Bending Stiffness of a Bimaterial Beam by the Approimation of OneDimensional of Laminated
More informationADVANCED DESIGN OF GLASS STRUCTURES
ADVANCED DESIGN OF GLASS STRUCTURES Lecture L13 Design of compressed members Viorel Ungureanu / Martina Eliášová European Erasmus Mundus Master Course Sustainable Constructions under Natural Hazards and
More informationAN UNLOADING AND RELOADING STRESSSTRAIN MODEL FOR CONCRETE CONFINED BY TIE REINFORCEMENTS
AN UNLOADING AND RELOADING STRESSSTRAIN MODEL FOR CONCRETE CONFINED BY TIE REINFORCEMENTS Junichi SAKAI 1 And Kazuhiko KAWASHIMA SUMMARY This paper presents a series of uniaxial compressive loading tests
More informationChapter 1 Introduction Concept of Stress
hapter 1 Introduction oncept of Stress INTRODUTION Review of Statics xial Stress earing Stress Torsional Stress 14 6 ending Stress W W L Introduction 11 Shear Stress W W Stress and Strain L y y τ xy
More informationFinite Element Analysis of Piezoelectric Cantilever
Finite Element Analysis of Piezoelectric Cantilever Nitin N More Department of Mechanical Engineering K.L.E S College of Engineering and Technology, Belgaum, Karnataka, India. Abstract Energy (or power)
More information6. NONLINEAR PSEUDOSTATIC ANALYSIS OF ADOBE WALLS
6. NONLINEAR PSEUDOSTATIC ANALYSIS OF ADOBE WALLS Blondet et al. [25] carried out a cyclic test on an adobe wall to reproduce its seismic response and damage pattern under inplane loads. The displacement
More informationResidual Stresses in Multilayer Ceramic Capacitors: Measurement and Computation
Jaap M. J. den Toonder Mem. ASME email: jaap.den.toonder@philips.com Philips Research Laboratories, Eindhoven, The Netherlands Christian W. Rademaker Philips Center for Industrial Technology, Eindhoven,
More informationSystem Capacity of Vintage Reinforced Concrete Moment Frame Culverts with No Overlay
DCT 252 System Capacity of Vintage Reinforced Concrete Moment Frame Culverts with No Overlay By Timothy Porter Thomas Schumacher August, 2015 Delaware Center for Transportation University of Delaware 355
More informationStrain sensors based on bragg gratings
IMEKO 20 th TC3, 3 rd TC16 and 1 st TC22 International Conference Cultivating metrological knowledge 27 th to 30 th November, 2007. Merida, Mexico. Strain sensors based on bragg gratings K. Haase Hottinger
More informationDELAMINATION CONTROL IN COMPOSITE BEAMS USING PIEZOELECTRIC ACTUATORS
DELAMINATION CONTROL IN COMPOSITE BEAMS USING PIEZOELECTRIC ACTUATORS L Iannucci 1, M S I Shaik Dawood 1,2,3, E Greenhalgh 1 and A K Ariffin 3 1 Aeronautics Department, Imperial College London, South Kensington
More informationENCE 455 Design of Steel Structures. III. Compression Members
ENCE 455 Design of Steel Structures III. Compression Members C. C. Fu, Ph.D., P.E. Civil and Environmental Engineering Department University of Maryland Compression Members Following subjects are covered:
More information8.3 Design of Base Plate for Thickness
8.3 Design o Base Plate or Thickness 8.3.1 Design o base plate or thickness (Elastic Design) Upto this point, the chie concern has been about the concrete oundation, and methods o design have been proposed
More informationTHE BENDING STIFFNESSES OF CORRUGATED BOARD
AMDVol. 145/MDVol. 36, Mechanics of Cellulosic Materials ASME 1992 THE BENDING STIFFNESSES OF CORRUGATED BOARD S. Luo and J. C. Suhling Department of Mechanical Engineering Auburn University Auburn,
More informationFinite Element Analysis of Composite Laminate By Using ABDH Matrix(Stiffness Matrix)
Finite Element Analysis of Composite Laminate By Using ABDH Matrix(Stiffness Matrix) Nikhil J. Chaudhari 1 Post Graduate Student Department of Mechanical Engineering Veermata Jijabai Technological Institute
More informationDesign and Analysis of Progressive Tool
Design and Analysis of Progressive Tool Ch.Mastanamma 1, K.Prasada Rao 2,Dr. M.Venkateswara Rao 3 1. PG Student, Department of Mechanical Engineering, Bapatla Engineering College, Bapatla, Guntur, India
More informationContinuous Beams  Flexibility Method
ontinuous eams  Flexibility Method Qu. Sketch the M diagram for the beam shown in Fig.. Take E = 200kN/mm 2. 50kN 60kNm = = 0kN/m D I = 60 50 40 x 0 6 mm 4 Fig. 60.0 23.5 D 25.7 6.9 M diagram in knm
More informationMicromeso draping modelling of noncrimp fabrics
Micromeso draping modelling of noncrimp fabrics Oleksandr Vorobiov 1, Dr. Th. Bischoff 1, Dr. A. Tulke 1 1 FTA Forschungsgesellschaft für Textiltechnik mbh 1 Introduction Noncrimp fabrics (NCFs) are
More information